- Open Access
The negative effect of ceria on the propene selectivity for isopropanol decomposition over phosphated and phosphate-free ceria/alumina catalysts
© Khalaf; licensee Springer. 2013
- Received: 7 October 2013
- Accepted: 11 November 2013
- Published: 20 November 2013
Consequences of loading level of ceria (5, 10 and 20-wt%) on the structural, textural and surface acid–base properties as well as the impacts on catalytic activity towards isopropanol decomposition on pure and phosphated alumina is described. The obtained results indicated that composites mainly kept γ–alumina structure and the addition of ceria and/or phosphate has no effect on the bulk structure of alumina. Textural characteristics show that the phosphated composites have higher surface area than phosphate free samples. Pyridine adsorption as followed by FTIR indicated the presence of Lewis acid sites with different strengths. Moreover, results of gas phase decomposition of isopropanol show a systematic inhibition in propene selectivity based on ceria ratio.
Active alumina, as one of the most common catalyst support, has a good performance in catalysis applications due to its physical and chemical properties (Levy et al. 1968). Alumina has various properties such as high specific surface area, surface acidity and defects in their crystalline structure that are the key factor in the wide range of applications. One of the most important factors in alumina utilization is thermal stability, which is a very important issue for processes running at high temperature (Chen et al. 2001). Therefore, the addition of some additives can improve the thermal stability of alumina catalysts, hold the surface area and improve the surface acidity (Shinjoh 2006; Ozawa 2006; Ozawa & Nishio 2004; Ersoy & Gunay 2004). Phosphates have been claimed to act as a support stabilizer (Gishti et al. 1984; Abbattista et al. 1990; Khalaf et al. 2007). Gishti et al. (1984; evidenced a stable effect of phosphate by studying the phase transitions of alumina in the range 673–1323 K. However, the surface area decreased with the increasing content of phosphate in alumina, even less than the blank sample after calcinated at 1073 K. Khalaf et al. 2007 also proved no surface area stabilization effect from phosphates in the case of the transition phase (spinel) aluminas.
Ceria possesses versatile acid–base properties, depending on the nature and temperature of the pretreatment. It may have high number of basic sites of weak or medium strength (Binet et al. 1999). Martin and Duprez found the following scale for the density of basic sites of some metal oxides CeO2 > MgO > ZrO2 > Al2O3 > SiO2 (Martin & Duprez 1997). Binet et al. (1999) also observed that ceria can chemisorb CO or pyridine, but the band positions strongly suggest that the Lewis acidity of ceria is significantly lower than that of zirconia or titania. In contrast to Lewis basicity, the Lewis acidity would decrease upon reduction of ceria.
Ceria and ceria-based materials has been widely employed as automotive three-way catalysts (TWC) for reducing the exhaust pollutants, fuel cell processes, oxygen permeation membrane systems, exhaust combustion catalysts, and catalytic wet oxidation (Yao & Yao 1984; Dos Santos et al. 2008; Bera et al. 2003; Khalil 2007). Cerium oxide can maintain large amounts of oxygen through the easy transition between Ce(IV) and Ce(III). This property is very useful in catalysis especially in oxidation reactions (Guimaraes et al. 2003). Nevertheless, pure ceria is poorly thermostable and undergoes rapid sintering under high temperature conditions, which leads to loss of oxygen buffer capacity and deactivation of the catalysts. The combination of two metals in an oxide can lead to novel structural and electronic properties of the final oxide, consequently modifying its catalytic activity and selectivity. Ceria-alumina mixed oxides are widely used as catalytic materials (Walter & Oldfield 1989; Niu et al. 1999; Sanchez-Valente et al. 2004).
In the present work, ceria-alumina as well as phosphate alumina modified with ceria have been prepared and characterized by several tools to gain an overview on the surface properties of these catalysts. In addition, the catalytic activities towards isopropanol decomposition for these composites have been explored.
The thermal events of ceria-alumina, xCeAl, and phosphate ceria-alumina, xCeAlP, samples are shown in Figure 1. It is cleared that, the increasing in the ceria loading levels resulted in increasing in the mass loss % (39.3, 50.0 and 54.0% for 5CeAl, 10CeAl and 20CeAl samples, respectively). This is logically, due to ceria losses mass higher than alumina. As for phosphated samples, one can noticed that there is no change in the mass loss % by the comparison between phosphated and phosphate-free samples. Thus, the phosphate ions have slightly effect on the mass loss % of phosphate samples. Only the main difference between xCeAl and xCeAlP is in the wider extended region for phosphated samples.
DTA results for all samples show two endothermic peaks, the first one appeared at low temperature (about 330 K) due to the elemination of adsorbet water, and the other one appeared at temperature higher than 480 K due to the decomposition of samples.
X-ray diffraction (XRD)
Nitrogen adsorption-desorption data
Data obtained from isotherms and BET plots of the samples under testing are cited in Table 1. From these data, it is clear that pure alumina sample has higher specific surface area (SBET = 187 m2g-1) than pure ceria (SBET = 12 m2g-1) which agree with previous data (Gishti et al. 1984). The addition of ceria into alumina, xCeAl, resulted in a gradual decrease in the surface area for the samples (SBET = 117, 53 and 50 m2g-1 for 5CeAl, 10CeAl and 20CeAl, respectively). For phosphated samples, there is a slightly effect of phosphate on the value of specific surface area in which the SBET values for xCeAlP are higher than that of xCeAl. These data agreed with those obtained from XRD results, which complied in Table 1, in which the variation in crystallite size has an effect on the specific surface area (Khalaf 2009). Hence, the noticeable increase in the SBET values for xCeAlP after phosphate addition could be attributed to the decrease in the crystallite size rather than any modification in the pore structure of the pure alumina. This result agrees with what has been reported in the literature (Larese et al. 2004).
PSD curves of the samples under study are illustrated in Figure 4. Examining these curves reveals that the addition of ceria and/or phosphate on to alumina causes a development in the porosity. In which, all samples are in micro-meso range. Moreover, the amount of mesopores in the phosphate-free samples is higher than that of phosphate samples.
FTIR spectra of adsorbed pyridine
Spectra taken from Py adsorption on 5CeAl, 10CeAl and 20CeAl samples at 300 K, show common feature of a gradual weakness in the intensity of the bands characteristic of the pure alumina. Py adsorption over phosphated alumina modified with ceria with different loading levels show similar spectra with phosphate free samples, so we only mention only one (xCeAl samples) to prevent the recurrence.
Conversion% of isopropanol as well as propene and acetone selectivities at 470 K
The results obtained from decomposition of isopropanol on γ-Al2O3 (Table 2) display mainly conversion of isopropanol to propene, whereas the formation of acetone is found to be very low (3.5%). The obtained results indicated that the selectivity of propene is 96.5%, thus, alumina surface have strong acidic sites, which is evident from the higher dehydration process than dehydrogenation, these results agree with that in literature (Khalaf et al. 2007). Alumina surface is known to acquire strong Lewis acid sites, which explain the high activity towards the dehydration pathway (Waqif et al. 1992). The results for pure ceria show that the dehydrogenation (87.5%) of isopropanol to acetone is higher than the dehydration (12.5%) process indicating the basicity of ceria surface. Ceria modified alumina samples, xCeAl, show that the incorporation of ceria into alumina resulted in a decrease in the propene selectivity from 96.5% for alumina to 74.4% for 20CeAl. This descending in propene selectivity% is analog with ascending of acetone selectivity% and could be attributed to the basicity of ceria. (Zaki et al. 1997) reported that ceria surface has Lewis base sites assuming a strong nucleophilic reactivity.
At the same time, the conversion of isopropanol and the selectivity towards propene formation for the phosphate catalysts, xCeAlP, is higher than that for the phosphate free catalysts. Knowing that isopropanol dehydrate to propene over acidic catalysts, this could explain such behavior of the phosphated catalysts. Furthermore, the obvious increase in the catalytic activity (% conversion) of the phosphated catalysts than phosphate free samples is in accordance with the data obtained from surface area measurement, in which the SBET for xCeAlP > SBET for xCeAl.
In conclusion, the addition of ceria and/or phosphate onto alumina with different loading levels causes a modification in the surface texture and porosity. The results show also that the ceria added to alumina is well dispersed on the surface of alumina and has no effect on the phase structure of pure alumina (γ-Al2O3 structure). Alumina, ceria and ceria-alumina composite show Lewis acid sites with different acidity strengths. Isopropanol decomposed to mainly propene by pure alumina and the addition of ceria decreases the amount of propene selectivity% and increases the acetone selectivity%, this is due to the basicity of ceria. Moreover, the phosphated samples have higher propene selectivity% than phosphate free samples indicating that the phosphate ions increase the acidity of the samples.
Two series of the catalysts under studying have been prepared. The first series is ceria doped alumina catalysts, abbreviated as xCeAl (where, x = 5, 10 and 20 wt%wt ceria) were prepared by coprecipitation method. The 1.5 molar solutions of Al(NO3)3.9H2O and Ce(NO3)3∙6H2O were prepared separately and then mixed in a volume proportions according to the final desired composition of catalysts. The resulting solution was stirred and heated to 350 K in a round bottom flask. The aqueous 1:1 M NH4OH solution was added drop wise to the nitrate solution under vigorous stirring until pH 8 was attained. After ageing for two hours, the excess solution was removed by filtration. Precipitate was washed repeatedly by distilled water followed by drying at 380 K for 12 h. The dried precursor was crushed to fine powder and calcined in the presence of static air at 873 K for 3 h.
The second series, xCeAlP (P refers to phosphate and x is the loading level of ceria, 5, 10 and 20 wt%), was obtained by impregnation of an aqueous solution of the impregnating (NH4)2HPO4 solution and held stirring for 1 h. The solution was adjusted to give 6 Wt% PO4-3 content. The excess water present was removed by evaporation at 380 K. The catalysts were obtained by calcination of the dried samples at 873 K for 3 h.
Apparatus and techniques
Thermogravimetric analysis (TGA) and deferential thermal analysis (DTA) were performed between room temperature and 1273 K in a static atmosphere of air, using Linseis STA PT 1600 thermogravimetric analyzer. The rate of heating was standardized at 10 K /min., and small portions (5–15 mg) of the sample were used in TG measurements.
X-ray powder diffractometry
where K is the crystallite shape constant (≈1), λ the radiation wavelength, β the line breadth (radians) and θ is the Bragg angle.
Nitrogen adsorption isotherm measurement
Full nitrogen adsorption/desorption isotherms at 77 K were obtained using a NOVA 2200, version 6.10 high-speed gas sorption analyzer (Quantachrome Corporation USA). The calcined samples were first out-gassed at 470 K for 1 h. Twenty four-point adsorption and desorption isotherms were obtained, from which BET surface areas were derived using standard and well-established methods (Sing et al. 1985; Webb & Orr 1997).
FTIR spectra for pyrodine adsorption
For pyridine (Py) adsorption on test samples a wafer of 15–20 mg/cm2 were mounted in a Pyrex vacuum cell fitted with CaF2 windows. The samples were pretreated at 700 K for 1 h in stream of O2 followed by evacuation at 700 K for 1 h, then cooled to room temperature to obtain the background IR spectra using Thermo scientific Nicolet 380 FTIR spectrophotometer. Then, 5 Torr Py (1 Torr = 133.32 Pa) were admitted at 300 k for 5 min., degassed for 5 min. at this temperature in order to remove the fraction physisorbed Py, and the spectra were then taken at room temperature.
Catalytic activity (isopropanol decomposition)
The catalytic activity experiments for isopropanol decomposition were carried out in a fluidized bed quartz flow reactor at atmospheric pressure. 0.2 g of the catalyst was activated in-situ at 670 K for 1 h in N2. isopropanol (Merck, product, 99.9%) was introduced at a flow rate of 15 ml min-1 into carrier gas flow of N2. The reaction products were analyzed by gas chromatography on 2-m long 1/8״ column packed with 10% Carbowax and Chromm WHP 80/100 using a model 3400 Varian Gas Chromatograph equipped with a flame ionization detector (FID).
Assoc. Prof. Hussein A. Khalaf: He was born in 1970 in Minia, Egypt. He received a B.Sc. degree of pure chemistry from Faculty of Science, Minia University, Egypt, 1992. He obtained a M.Sc.(1999) and Ph.D (2005) degrees in Physical chemistry (surface and catalysis) from Minia University, Egypt, under the supervision of Professors Seham A. Mansour, Nasr E. Fouad, Ahmed K. Nohman and Gamal A. Mekhemer. And he is currently working as associated prof. at Omar El-Mukhtar University, Libya.
- Levy RM, Bauer DJ, Roth JF: Effect of Thermal Aging on the Physical Properties of Activated Alumina. Ind Eng Chem Prod Res Dev 1968, 7: 217. 10.1021/i360027a013View ArticleGoogle Scholar
- Chen X, Liu Y, Niu G, Yang Z, Bian M, He A: High temperature thermal stabilization of alumina modified by lanthanum species. Appl Catal A Gen 2001, 205: 159. 10.1016/S0926-860X(00)00575-5View ArticleGoogle Scholar
- Shinjoh H: Rare earth metals for automotive exhaust catalysts. J Alloys Compd 2006, 408: 1061.View ArticleGoogle Scholar
- Ozawa M: Thermal stabilization of catalytic compositions for automobile exhaust treatment through rare earth modification of alumina nanoparticle support. J Alloys Compd 2006, 408: 1090.View ArticleGoogle Scholar
- Ozawa M, Nishio Y: Thermal stabilization of γ-alumina with modification of lanthanum through homogeneous precipitation. J Alloys Compd 2004, 374: 397. 10.1016/j.jallcom.2003.11.032View ArticleGoogle Scholar
- Ersoy B, Gunay V: Effects of La2O3 addition on the thermal stability of γ-Al2O3 gels. Ceram Int 2004, 30: 163. 10.1016/S0272-8842(03)00084-1View ArticleGoogle Scholar
- Gishti K, Iannibello A, Marengo S, Morellili G, Tittarelli P: On the role of phosphate anion in the MoO3-Al2O3 based catalysts. Appl Catal 1984, 12: 381. 10.1016/S0166-9834(00)81675-9View ArticleGoogle Scholar
- Abbattista F, Delmastro A, Gozzelino G: Effect of phosphate ions on the surface chemistry and microstructure of amorphous alumina. J Chem Soc Faraday Trans 1990, 86: 3653. 10.1039/ft9908603653View ArticleGoogle Scholar
- Khalaf HA, Mekhemer GAH, Nohman AK, Mansour SAA: Phosphated Alumina Catalysts: Surface Properties and Reactivity towards 2-PrOH Decomposition. Monatsh Chem 2007, 138: 641. 10.1007/s00706-007-0674-6View ArticleGoogle Scholar
- Binet C, Daturi M, Lavalley JC: IR study of polycrystalline ceria properties in oxidised and reduced states. Catal Today 1999, 50: 207. 10.1016/S0920-5861(98)00504-5View ArticleGoogle Scholar
- Martin D, Duprez D: Evaluation of the acid-base surface properties of several oxides and supported metal catalysts by means of model reactions. J Mol Catal A Chem 1997, 118: 113. 10.1016/S1381-1169(96)00371-8View ArticleGoogle Scholar
- Yao HC, Yao YFY: Ceria in automotive exhaust catalysts: I. Oxygen storage. J Catal 1984, 86: 254. 10.1016/0021-9517(84)90371-3View ArticleGoogle Scholar
- Dos Santos ML, Lima RC, Riccardi CS, Tranquilin RL, Bueno PR, Varela JA, Longo E: Preparation and characterization of ceria nanospheres by microwave-hydrothermal method. Mater Lett 2008, 62: 4509. 10.1016/j.matlet.2008.08.011View ArticleGoogle Scholar
- Bera P, Gayen A, Hegde MS, Lalla NP, Spadaro L, Frusteri , Arena F: Promoting Effect of CeO2 in Combustion Synthesized Pt/CeO2 Catalyst for CO Oxidation. J Phys Chem B 2003, 107: 6122. 10.1021/jp022132fView ArticleGoogle Scholar
- Khalil KMS: Synthesis and characterization of mesoporous ceria/alumina nanocomposite materials via mixing of the corresponding ceria and alumina gel precursors. J Colloid Interface Sci 2007, 307: 172. 10.1016/j.jcis.2006.11.039View ArticleGoogle Scholar
- Guimaraes AL, Dieguez LC, Schmal M: Surface Sites of Pd/CeO2/Al2O3 Catalysts in the Partial Oxidation of Propane. J Phys Chem B 2003, 107: 4311. 10.1021/jp0270194View ArticleGoogle Scholar
- Walter TH, Oldfield E: Magic angle spinning oxygen-17 NMR of aluminum oxides and hydroxides. J Phys Chem 1989, 93: 6744. 10.1021/j100355a034View ArticleGoogle Scholar
- Niu G, Huang Y, Chen X, He J, Liu Y, He A: Thermal and hydrothermal stability of siliceous Y zeolite and its application to high-temperature catalytic combustion. Appl Catal B Environ 1999, 21: 63. 10.1016/S0926-3373(99)00009-0View ArticleGoogle Scholar
- Sanchez-Valente J, Bokhimi X, Toledo JA: Synthesis and catalytic properties of nanostructured aluminas obtained by sol–gel method. Appl Catal A Gen 2004, 264: 175. 10.1016/j.apcata.2003.12.041View ArticleGoogle Scholar
- Ai M: The activity of WO3-based mixed-oxide catalysts: I. Acidic properties of WO3-based catalysts and correlation with catalytic activity. J Catal 1977, 49: 305. 10.1016/0021-9517(77)90270-6View ArticleGoogle Scholar
- Abdellah O, Coudurier G, Vedrine JC: Acid–base properties of metallic oxide catalysts studied by conversion of propan-2-ol. J Chem Soc Farad Trans 1993, 89: 3151. 10.1039/ft9938903151View ArticleGoogle Scholar
- López I, Valdés-Solís T, Marbán G: The synthesis of high surface area cerium oxide and cerium oxide/silica nanocomposites by the silica aquagel-confined co-precipitation technique. Microporous Mesoporous Mater 2010, 127: 198. 10.1016/j.micromeso.2009.07.014View ArticleGoogle Scholar
- Marcu IC, Urlan MN, Redey A, Sandulescu I: Phosphated ceria, selective catalysts for oxidative dehydrogenation of isobutene. C R Chimie 2010, 13: 365. 10.1016/j.crci.2009.12.007View ArticleGoogle Scholar
- JCPDS, International Centre for Diffraction Data, PCPDFWIN: JCPDS-ICDD. 1995.Google Scholar
- Silversand AFA, Ingemar CU, Odembrand : Combustion of methane over a Pd-Al2O3/SiO2 catalyst, catalyst activity and stability. Appl Catal 1997, 153: 157. 10.1016/S0926-860X(96)00328-6View ArticleGoogle Scholar
- Johnson MFL: Surface area stability of aluminas. J Catal 1990, 123: 245. 10.1016/0021-9517(90)90173-HView ArticleGoogle Scholar
- Klug HP, Alexander LE: X-ray Diffraction Procedures, vol 9. New York: Wiley; 1970:490.Google Scholar
- Brunauer S, Emmett PH, Teller T: Adsorption of Gases in Multimolecular Layers. J Am Chem Soc 1938, 60: 309. 10.1021/ja01269a023View ArticleGoogle Scholar
- Gregg SJ, Sing KSW: Adsorption, Surface Area and Porosity. London: Academic Press; 1982.Google Scholar
- Sing KSW, Everett DH, Haul RAW, Moscou L, Pierotti RA, Rouquerol J, Siemieniewska T: Reporting physisorption data for gas/solid systems with special reference to the determination of surface area and porosity (Recommendations 1984). Pure Appl Chem 1985, 57: 603. 10.1351/pac198557040603View ArticleGoogle Scholar
- Khalaf HA: Textural properties of sulfated iron hydroxide promoted with aluminum. Monatsh Chem 2009, 140: 669. 10.1007/s00706-009-0118-6View ArticleGoogle Scholar
- Larese C, Cabello Galisteo F, Granados ML, Mariscal R, Fierro JLG, Lambrou PS, Efstathiou AM: Effects of the CePO4 on the oxygen storage and release properties of CeO2 and Ce0.8Zr0.2O2 solid solution. J Catal 2004, 226: 443. 10.1016/j.jcat.2004.06.013View ArticleGoogle Scholar
- Mikhail RS, Sheb F: Adsorption in relation to pore structures of silicas II. Water vapor adsorption on wide-pore and microporous silica gels. J Colloid Interface Sci 1970, 34: 65. 10.1016/0021-9797(70)90259-6View ArticleGoogle Scholar
- Ismail HM, Hussein GAM: Texture properties of yttrium oxides generated from different inorganic precursors. Powder Techn 1996, 87: 87. 10.1016/0032-5910(95)03060-3View ArticleGoogle Scholar
- Mekhemer GAH, Nohman AKH, Fouad NE, Khalaf HA: Surface to bulk characterization of phosphate modified aluminas. Colloid Surf A 2000, 161: 439. 10.1016/S0927-7757(99)00123-5View ArticleGoogle Scholar
- Zaki MI, Hussein GAM, Mansour SAA, El-Ammawy HA: Adsorption and surface reactions of pyridine on pure and doped ceria catalysts as studied by infrared spectroscopy. J Mol Catal 1989, 51: 209. 10.1016/0304-5102(89)80101-4View ArticleGoogle Scholar
- Waqif M, Baachelier J, Saur O, Lavalley JC: Acidic properties and stability of sulfate-promoted metal oxides. J Mol Catal 1992, 72: 127. 10.1016/0304-5102(92)80036-GView ArticleGoogle Scholar
- Zaki MI, Hussein GAM, Mansour SAA, Ismail HM, Mekhemer GAH: Ceria on silica and alumina catalysts: dispersion and surface acid-base properties as probed by X-ray diffractometry, UV-Vis diffuse reflectance and in situ IR absorption studies. Colloid and Surf A 1997, 127: 47. 10.1016/S0927-7757(96)03943-XView ArticleGoogle Scholar
- Frank W, et al.: Powder Diffraction File for Inorganic Phase. Philaddphia PA: International Center for Diffraction Data; 1981.Google Scholar
- Webb PA, Orr C: Analytical methods in fine particle technology. Norcross, GA USA: Micromeritics Instrument Corp; 1997:156-159.Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.